INCLUSIONS IN CONTINUOUS CASTING OF STEEL
Lifeng Zhang (Dr.), Brian G. Thomas (Prof.)
140 Mech. Engr. Buldg., 1206 W. Green St.
Univ. of Illinois at Urbana-Champaign Urbana, IL61801, U.S.A.
Tel: 1-217-244-4656 Fax: 1-217-244-6534 email@example.com, firstname.lastname@example.org
ABSTRACT This paper first reviews the sources of inclusions in continuous casting of steel including both indigenous and exogenous inclusions, focusing on reoxidation, slag entrainment, lining erosion and inclusion agglomeration on linings. Secondly, the resulting defects in continuous cast steel products are reviewed, such as flange cracked cans, slag spots, and line defects on the surface of rolled sheet. Thirdly, the current state-of-the-art in the evaluation of steel cleanliness is summarized, discussing over 30 different methods including direct and indirect methods. Finally, this paper reviews operating practices to improve steel cleanliness at the tundish and continuous caster. Key Words: Steel, Inclusions, Defects, Slab Caster, Plant Measurement, Review, Detection Methods
INCLUSIONS AND DEFECTS 1. Introduction
The ever-increasing demands for high quality have made the steelmaker increasingly aware of product cleanliness requirements. Non-metallic inclusions are a significant problem in cast steels that can lead to excessive casting repairs or rejected castings. Ginzburg and Ballas reviewed the defects in cast slabs and hot rolled products, many of which are related to inclusions. 1) The mechanical behavior of steel is controlled to a large degree by the volume fraction, size, distribution, composition and morphology of inclusions and precipitates, which act as stress raisers. The inclusion size distribution is particularly important, because large macroinclusions are the most harmful to mechanical properties. Sometimes a catastrophic defect is caused by just a single large inclusion in a whole steel heat. Though the large inclusions are far outnumbered by the small ones, their total volume fraction may be larger.2)
Ductility is appreciably decreased by increasing amounts of either oxides or sulphides. 3) Fracture toughness decreases when inclusions are present in higher-strength lower-ductility alloys. Similar property degradation from inclusions is observed in tests that reflect slow, rapid, or cyclic strain rates, such as creep, impact, and fatigue testing. 3) Figure 1 shows that inclusions cause voids, which can induce cracks. 4) Large exogenous inclusions may cause trouble in the form of inferior surface, poor
L. Zhang & BG Thomas: XXIV National Steelmaking Symposium, Morelia, Mich, Mexico, 26-28, Nov.2003, pp. 138-183.
polishability, reduced resistence to corrosion, and in exceptional cases, slag lines and laminations. 5) Inclusions also lower resistance to HIC (Hydrogen Induced Cracks). 6) The source of most fatigue problems in bearing steel are hard and brittle oxides, especially large alumina particles over 30m. 7-10) 11) Figure 2 7) indicates that lowering the amount of large inclusions by lowering the oxygen content to 3-6ppm has extended bearing life by almost 30 times in comparison with steels with 20 ppm oxygen. To avoid these problems, the size and frequency of detrimental inclusions must be carefully controlled. Especially there should be no inclusions in the casting above a critical size. Table I shows some typical restrictions on inclusions in different steel application. 12)
Table 1. Typical steel cleanliness requirements reported for various steel grades
Steel product Maximum impurity fraction Maximum inclusion size Automotive & deep-drawing Sheet
[C]30ppm, [N]30ppm 13) 100m 13, 14)
Drawn and Ironed cans [C]30ppm, [N]30ppm, T.O.20ppm 13)
Line pipe [S]30ppm 15), [N]35ppm, T.O.30ppm 16), [N]50ppm17)
Ball Bearings T.O.10ppm15, 18) 15m16, 18) Tire cord [H]2ppm, [N]40ppm,
T.O.15ppm16) 10m16) 20m14)
Heavy plate steel [H]2ppm, [N]30-40ppm, T.O.20ppm16)
Single inclusion 13m13) Cluster 200m13)
Wire [N]60ppm, T.O.30ppm16) 20m16)
Although the solidification morphology of inclusions is important in steel castings, the morphology of inclusions in wrought products is largely controlled by their mechanical behavior during steel processing, i.e., whether they are hard or soft relative to the steel matrix. The behavior of different types of inclusions during deformation is schematically illustrated in figure 3. 19) Stringer formation, type (b) and (c), increases the directionality of mechanical properties, adversely affecting toughness and ductility in particular. The worst inclusions for toughness and ductility, particularly in through-thickness direction properties of flat-rolled product, are those deforming with the matrix, like (d) in Fig. 3.
Fig.1 Effect of inclusion deformation on linking between adjacent voids
Fig.2 Relation between fatigue life and oxygen content of bearing steels
Fig. 3 Schematic representation of inclusions morphologies before and after deformation. 19)
Steel cleanliness is an important topic that has received much attention in the literature. An
extensive review on clean steel by Kiessling in 1980 summarized inclusion and trace element control and evaluation methods, especially for ingots. 20) More recent reviews of this topic have been made by Mu and Holappa (1992) 21) and by Cramb (1999) 14) which added extensive thermodynamic considerations. McPherson and McLean (1992) reviewed non-metallic inclusions in continuously casting steel, focusing on the inclusion types (oxides, sulfides, oxysulfides, nitrides and carbonitrides), inclusion distributions and methods to detect inclusions in this process.22) Zhang and Thomas (2003) reviewed detection methods of inclusions, and operating practices to improve steel cleanliness at the ladle, tundish and continuous caster. 12) The rest of this report is an extensive review on inclusions in steel continuous casting, their sources, morphology, formation mechanisms, detection methods, and the effect of various continuous casting operations. 2. Inclusions in Steel
Non-metallic inclusions in steel are termed as indigenous inclusions and exogenous inclusions according to their sources.
2.1 Indigenous Inclusions
Indigenous inclusions are deoxidation products or precipitated inclusions during cooling and solidification of steel.
Fig. 4 Dendritic and clustered alumina inclusions (left), and coral-like alumina inclusions (right)
formed during deoxidation of pure iron 42)
1) Deoxidation products 23-29) 30-34) 6, 35-41) Alumina (Al2O3) inclusions in LCAK steel, and silica (SiO2) inclusions in Si-killed steel are
generated by the reaction between the dissolved oxygen and the added aluminum and silicon deoxidants are typical deoxidation inclusions. Alumina inclusions are dendritic when formed in a high oxygen environment, as pictured in figure 442).
Cluster-type alumina inclusions from deoxidation or reoxidation, 42, 43) as shown in figure 543), are typical of aluminum killed steels. Alumina inclusions easily form three dimensional clusters via collision and aggregation due to their high interfacial energy. Individual inclusions in the cluster can be 1 -5 microns in diameter 39-41).Before collision, breakup or aggregation with other particles, they may be in the shape of flower plate44) or (aggregated) polyhedral inclusions45, 46) (figure 644)). Alternatively coral-like alumina inclusions (figure 442)) are believed to result from Ostwald-ripening 39-41, 47-51) of originally dendrtic or clustered alumina inclusions. Fig. 5 Alumina cluster during deoxidation
of low carbon steel by aluminum 43)
Fig. 6 Alumina inclusions formed during the deoxidation of LCAK steel (left: flower-like plate
alumina; right: aggregation of small polyhedral particles) 44) Silica inclusions are generally spherical owing to being in a liquid or glassy state in the molten
steel. Silica can also agglomerate into clusters as shown in figure 745, 52).
Fig. 7 Agglomeration of round silica inclusions 45) 52)
2) Precipitated inclusions form during cooling and solidification of the steel 10, 33, 53-59)
During cooling, the concentration of dissolved oxygen/nitrogen/sulfur in the liquid becomes larger while the solubility of those elements decreases. Thus inclusions such as alumina59), silica, AlN54), and
sulphide precipitate. Sulphides form interdendritically during solidification, and often nucleate on oxides already present in the liquid steel. 60) These inclusions are normally small (3000.1
Inclusion diameter (m)
Start of RH End of RH Tundish Slab
Fig. 9 Size distribution of large inclusions in a continuous casting slab 61)
Exogenous inclusions have the following common characteristics:
i). Large size: Inclusions from refractory erosion are generally larger than those from slag entrainment. 62)
ii). Compound composition/ multiphase, cause by the following phenomena: - Due to the reaction between molten steel and SiO2, FeO, and MnO in the slag and lining
refractory, the generated Al2O3 inclusions may stay on their surface;
- As exogenous inclusions move, due to their large size, they may entrap deoxidation inclusions such as Al2O3 on their surface (Fig.10 right and Fig.11 right);
- Exogenous inclusions act as heterogeneous nucleus sites for precipitation of new inclusions during their motion in molten steel (Fig.11 left);
- Slag or reoxidation inclusions may react with the